  
data_1m_0m 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'H20 K5 N O45 Se6 U4' 
_chemical_formula_weight          2375.55 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'K'  'K'   0.2009   0.2494 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Se'  'Se'  -0.0929   2.2259 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'U'  'U'  -9.6767   9.6646 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'N'  'N'   0.0061   0.0033 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting           'Monoclinic'
_symmetry_space_group_name_H-M   'C2/c'
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, y, -z+1/2' 
 'x+1/2, y+1/2, z' 
 '-x+1/2, y+1/2, -z+1/2' 
 '-x, -y, -z' 
 'x, -y, z-1/2' 
 '-x+1/2, -y+1/2, -z' 
 'x+1/2, -y+1/2, z-1/2' 
 
_cell_length_a                    20.290(4) 
_cell_length_b                    10.3800(18) 
_cell_length_c                    21.436(4) 
_cell_angle_alpha                 90.00 
_cell_angle_beta                  103.446(3) 
_cell_angle_gamma                 90.00 
_cell_volume                      4391.0(13) 
_cell_formula_units_Z             4 
_cell_measurement_temperature     210(2) 
_cell_measurement_reflns_used     9914
_cell_measurement_theta_min       2.49
_cell_measurement_theta_max       35.66
 
_exptl_crystal_description        'plate' 
_exptl_crystal_colour             'yellow-green' 
_exptl_crystal_size_max           0.25 
_exptl_crystal_size_mid           0.16 
_exptl_crystal_size_min           0.09 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.593 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              4216 
_exptl_absorpt_coefficient_mu     20.278 
_exptl_absorpt_correction_type    'multi-scan'
_exptl_absorpt_correction_T_min   0.1587
_exptl_absorpt_correction_T_max   0.4275
_exptl_absorpt_process_details    'SADABS; Bruker, 2007'
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       210(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker APEX-II CCD'
_diffrn_measurement_method        'φ and ω scans'
_diffrn_detector_area_resol_mean  ? 
_diffrn_reflns_number             33030 
_diffrn_reflns_av_R_equivalents   0.0548 
_diffrn_reflns_av_sigmaI/netI     0.0429 
_diffrn_reflns_limit_h_min        -30 
_diffrn_reflns_limit_h_max        30 
_diffrn_reflns_limit_k_min        -15 
_diffrn_reflns_limit_k_max        15 
_diffrn_reflns_limit_l_min        -32 
_diffrn_reflns_limit_l_max        32 
_diffrn_reflns_theta_min          1.95 
_diffrn_reflns_theta_max          32.50 
_reflns_number_total              7944 
_reflns_number_gt                 6405 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection       'Bruker APEX2'
_computing_cell_refinement       'Bruker SAINT'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_molecular_graphics     ? 
_computing_publication_material   ? 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0334P)²+0.0000P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     mixed 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          7944 
_refine_ls_number_parameters      306 
_refine_ls_number_restraints      13 
_refine_ls_R_factor_all           0.0390 
_refine_ls_R_factor_gt            0.0268 
_refine_ls_wR_factor_ref          0.0685 
_refine_ls_wR_factor_gt           0.0657 
_refine_ls_goodness_of_fit_ref    1.030 
_refine_ls_restrained_S_all       1.040 
_refine_ls_shift/su_max           0.000 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
U1 U 0.788786(8) 0.339121(14) 0.297341(8) 0.01423(4) Uani 1 1 d . . . 
U2 U 0.585894(9) 0.252956(15) 0.047975(8) 0.01623(4) Uani 1 1 d . . . 
Se1 Se 0.86684(2) 0.66241(4) 0.28249(2) 0.01491(9) Uani 1 1 d . . . 
Se2 Se 0.70933(2) 0.49973(4) 0.14020(2) 0.01499(9) Uani 1 1 d . . . 
Se3 Se 0.56264(2) -0.10793(4) 0.06678(2) 0.01800(9) Uani 1 1 d . . . 
K1 K 0.70613(8) 0.66516(12) 0.39448(7) 0.0408(3) Uani 1 1 d . . . 
K2 K 0.43450(7) 0.31267(14) 0.16243(7) 0.0402(3) Uani 1 1 d . . . 
K3 K 1.0000 0.45833(18) 0.2500 0.0552(6) Uani 1 2 d S . . 
O1 O 0.8135(2) 0.2426(3) 0.23893(17) 0.0243(7) Uani 1 1 d . . . 
O2 O 0.7066(2) 0.6565(3) 0.13271(17) 0.0232(7) Uani 1 1 d . . . 
O3 O 0.76367(19) 0.4374(3) 0.35480(16) 0.0218(7) Uani 1 1 d . . . 
O4 O 0.81998(19) 0.7434(3) 0.22272(17) 0.0225(7) Uani 1 1 d . . . 
O5 O 0.84342(18) 0.6982(3) 0.34893(16) 0.0204(7) Uani 1 1 d . . . 
O6 O 0.7713(2) 0.4372(3) 0.11447(19) 0.0279(8) Uani 1 1 d . . . 
O7 O 0.51462(19) 0.3064(3) 0.07445(19) 0.0261(8) Uani 1 1 d . . . 
O8 O 0.65774(19) 0.2036(4) 0.02079(18) 0.0281(8) Uani 1 1 d . . . 
O9 O 0.85402(19) 0.5088(3) 0.26689(18) 0.0247(8) Uani 1 1 d . . . 
O10 O 0.71335(18) 0.4619(3) 0.21564(16) 0.0226(7) Uani 1 1 d . . . 
O11 O 0.5983(2) -0.1718(3) 0.13638(19) 0.0286(8) Uani 1 1 d . . . 
O12 O 0.48700(19) -0.1743(3) 0.04643(17) 0.0257(8) Uani 1 1 d . . . 
O13 O 0.63656(18) 0.4472(3) 0.09601(17) 0.0236(7) Uani 1 1 d . . . 
O14 O 0.5512(2) 0.0464(3) 0.07707(18) 0.0268(8) Uani 1 1 d . . . 
O15 O 0.6076(2) -0.1294(4) 0.01469(19) 0.0330(9) Uani 1 1 d . . . 
O16 O 0.94523(18) 0.6961(4) 0.28594(19) 0.0267(8) Uani 1 1 d . . . 
O17 O 0.5727(3) 0.4170(4) -0.0337(2) 0.0450(12) Uani 1 1 d D . . 
H17A H 0.558(4) 0.505(4) -0.025(4) 0.067 Uiso 1 1 d D . . 
H17B H 0.539(3) 0.408(7) -0.0759(19) 0.067 Uiso 1 1 d D . . 
O18 O 0.6362(2) 0.6375(4) -0.0395(2) 0.0338(9) Uani 1 1 d D . . 
H18A H 0.680(2) 0.656(6) -0.049(4) 0.051 Uiso 1 1 d D . . 
H18B H 0.628(4) 0.714(4) -0.015(3) 0.051 Uiso 1 1 d D . . 
O19 O 0.7599(2) 0.5295(5) -0.0115(2) 0.0387(10) Uani 1 1 d D . . 
H19A H 0.760(4) 0.465(6) 0.022(3) 0.058 Uiso 1 1 d D . . 
H19B H 0.798(3) 0.557(7) -0.030(4) 0.058 Uiso 1 1 d D . . 
O20 O 0.4111(3) 0.0504(6) 0.1341(3) 0.0612(15) Uani 1 1 d D . . 
H20A H 0.434(5) 0.028(9) 0.099(3) 0.092 Uiso 1 1 d D . . 
H20B H 0.399(5) -0.043(3) 0.129(5) 0.092 Uiso 1 1 d D . . 
O21 O 0.4741(4) 0.4422(7) -0.1395(3) 0.078(2) Uani 1 1 d D . . 
H21A H 0.513(2) 0.434(11) -0.163(2) 0.118 Uiso 1 1 d D . . 
H21B H 0.438(2) 0.435(10) -0.181(2) 0.118 Uiso 1 1 d D . . 
N1 N 0.4368(6) 0.6592(10) 0.2017(6) 0.0443(13) Uani 0.50 1 d PD . . 
O22 O 0.4024(5) 0.5477(8) 0.2014(5) 0.0443(13) Uani 0.50 1 d PD . . 
O23 O 0.4867(5) 0.6910(7) 0.2527(7) 0.0443(13) Uani 0.50 1 d P . . 
O24 O 0.4233(5) 0.7589(8) 0.1619(5) 0.0443(13) Uani 0.50 1 d P . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
U1 O3 1.763(3) . ? 
U1 O1 1.765(3) . ? 
U1 O4 2.366(3) 4_645 ? 
U1 O9 2.384(3) . ? 
U1 O11 2.402(4) 4_655 ? 
U1 O2 2.405(3) 4_645 ? 
U1 O10 2.406(3) . ? 
U1 K1 4.4974(16) . ? 
U1 K1 4.5140(16) 4_645 ? 
U2 O7 1.761(4) . ? 
U2 O8 1.767(4) . ? 
U2 O12 2.358(3) 5_655 ? 
U2 O14 2.384(3) . ? 
U2 O13 2.386(3) . ? 
U2 O5 2.406(3) 4_645 ? 
U2 O17 2.412(4) . ? 
U2 K1 4.2117(17) 4_645 ? 
U2 K2 4.3984(15) . ? 
Se1 O16 1.613(4) . ? 
Se1 O9 1.638(3) . ? 
Se1 O4 1.639(3) . ? 
Se1 O5 1.645(3) . ? 
Se1 K2 3.5473(15) 3 ? 
Se1 K3 3.6258(13) . ? 
Se2 O6 1.621(4) . ? 
Se2 O2 1.635(3) . ? 
Se2 O10 1.648(3) . ? 
Se2 O13 1.650(3) . ? 
Se3 O15 1.613(4) . ? 
Se3 O11 1.639(4) . ? 
Se3 O14 1.641(3) . ? 
Se3 O12 1.646(4) . ? 
K1 O24 2.799(10) 2_655 ? 
K1 O3 2.853(4) . ? 
K1 O6 2.874(4) 4_655 ? 
K1 O19 2.884(5) 6_566 ? 
K1 O1 2.907(4) 4_655 ? 
K1 O22 2.908(9) 2_655 ? 
K1 O8 2.959(4) 4_655 ? 
K1 N1 3.144(12) 2_655 ? 
K1 O5 3.177(4) . ? 
K1 O8 3.374(4) 6_566 ? 
K1 U2 4.2117(17) 4_655 ? 
K2 O22 2.707(8) . ? 
K2 O16 2.718(4) 4_645 ? 
K2 O18 2.741(5) 5_665 ? 
K2 O7 2.762(4) . ? 
K2 O20 2.806(6) . ? 
K2 O16 2.873(4) 3_445 ? 
K2 O4 2.997(4) 3_445 ? 
K2 O21 3.253(9) 5_665 ? 
K2 Se1 3.5472(15) 3_445 ? 
K2 K2 4.064(3) 2_655 ? 
K2 K3 4.202(2) 3_445 ? 
K3 O23 2.789(8) 3_545 ? 
K3 O23 2.789(8) 4_645 ? 
K3 O20 2.873(7) 4_655 ? 
K3 O20 2.873(6) 3 ? 
K3 O16 2.884(4) . ? 
K3 O16 2.884(4) 2_755 ? 
K3 O24 2.984(9) 3_545 ? 
K3 O24 2.984(9) 4_645 ? 
K3 O9 3.111(4) . ? 
K3 O9 3.111(4) 2_755 ? 
K3 N1 3.426(11) 3_545 ? 
K3 N1 3.426(11) 4_645 ? 
O1 K1 2.907(4) 4_645 ? 
O2 U1 2.405(3) 4_655 ? 
O4 U1 2.366(3) 4_655 ? 
O4 K2 2.997(4) 3 ? 
O5 U2 2.406(3) 4_655 ? 
O6 K1 2.874(4) 4_645 ? 
O8 K1 2.959(4) 4_645 ? 
O8 K1 3.374(4) 6_565 ? 
O11 U1 2.402(4) 4_645 ? 
O12 U2 2.358(3) 5_655 ? 
O16 K2 2.718(4) 4_655 ? 
O16 K2 2.873(4) 3 ? 
O17 H17A 0.99(2) . ? 
O17 H17B 1.00(2) . ? 
O18 K2 2.741(5) 5_665 ? 
O18 H18A 0.98(2) . ? 
O18 H18B 0.99(2) . ? 
O19 K1 2.884(5) 6_565 ? 
O19 H19A 0.99(2) . ? 
O19 H19B 1.00(2) . ? 
O20 K3 2.873(6) 3_445 ? 
O20 H20A 1.00(2) . ? 
O20 H20B 1.00(2) . ? 
O21 K2 3.253(9) 5_665 ? 
O21 H21A 1.05(2) . ? 
O21 H21B 1.01(2) . ? 
N1 O24 1.329(14) . ? 
N1 O23 1.346(17) . ? 
N1 O22 1.351(12) . ? 
N1 O23 1.663(17) 2_655 ? 
N1 K1 3.144(12) 2_655 ? 
N1 K3 3.426(11) 3_455 ? 
O22 K1 2.908(9) 2_655 ? 
O23 O23 0.577(19) 2_655 ? 
O23 N1 1.663(17) 2_655 ? 
O23 K3 2.790(8) 3_455 ? 
O24 K1 2.799(10) 2_655 ? 
O24 K3 2.984(9) 3_455 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O3 U1 O1 179.13(16) . . ? 
O3 U1 O4 87.76(15) . 4_645 ? 
O1 U1 O4 92.29(15) . 4_645 ? 
O3 U1 O9 91.90(14) . . ? 
O1 U1 O9 87.56(14) . . ? 
O4 U1 O9 144.50(13) 4_645 . ? 
O3 U1 O11 90.29(15) . 4_655 ? 
O1 U1 O11 90.18(16) . 4_655 ? 
O4 U1 O11 143.98(13) 4_645 4_655 ? 
O9 U1 O11 71.51(13) . 4_655 ? 
O3 U1 O2 89.77(14) . 4_645 ? 
O1 U1 O2 91.07(14) . 4_645 ? 
O4 U1 O2 71.44(13) 4_645 4_645 ? 
O9 U1 O2 144.06(13) . 4_645 ? 
O11 U1 O2 72.59(13) 4_655 4_645 ? 
O3 U1 O10 87.93(14) . . ? 
O1 U1 O10 91.27(15) . . ? 
O4 U1 O10 71.43(12) 4_645 . ? 
O9 U1 O10 73.08(13) . . ? 
O11 U1 O10 144.46(12) 4_655 . ? 
O2 U1 O10 142.86(13) 4_645 . ? 
O3 U1 K1 16.63(11) . . ? 
O1 U1 K1 162.50(12) . . ? 
O4 U1 K1 88.14(9) 4_645 . ? 
O9 U1 K1 82.04(8) . . ? 
O11 U1 K1 99.72(9) 4_655 . ? 
O2 U1 K1 105.60(9) 4_645 . ? 
O10 U1 K1 72.29(9) . . ? 
O3 U1 K1 159.93(11) . 4_645 ? 
O1 U1 K1 19.32(13) . 4_645 ? 
O4 U1 K1 83.37(9) 4_645 4_645 ? 
O9 U1 K1 85.08(9) . 4_645 ? 
O11 U1 K1 107.41(10) 4_655 4_645 ? 
O2 U1 K1 104.29(8) 4_645 4_645 ? 
O10 U1 K1 72.19(9) . 4_645 ? 
K1 U1 K1 144.37(2) . 4_645 ? 
O7 U2 O8 178.47(17) . . ? 
O7 U2 O12 89.28(16) . 5_655 ? 
O8 U2 O12 91.00(16) . 5_655 ? 
O7 U2 O14 83.36(15) . . ? 
O8 U2 O14 98.17(16) . . ? 
O12 U2 O14 75.45(12) 5_655 . ? 
O7 U2 O13 84.18(15) . . ? 
O8 U2 O13 94.68(16) . . ? 
O12 U2 O13 141.69(12) 5_655 . ? 
O14 U2 O13 140.43(12) . . ? 
O7 U2 O5 97.88(15) . 4_645 ? 
O8 U2 O5 82.71(15) . 4_645 ? 
O12 U2 O5 145.84(12) 5_655 4_645 ? 
O14 U2 O5 72.33(12) . 4_645 ? 
O13 U2 O5 72.44(12) . 4_645 ? 
O7 U2 O17 92.89(18) . . ? 
O8 U2 O17 85.78(19) . . ? 
O12 U2 O17 71.33(13) 5_655 . ? 
O14 U2 O17 146.61(13) . . ? 
O13 U2 O17 71.36(13) . . ? 
O5 U2 O17 140.83(13) 4_645 . ? 
O7 U2 K1 144.64(13) . 4_645 ? 
O8 U2 K1 35.57(13) . 4_645 ? 
O12 U2 K1 124.22(10) 5_655 4_645 ? 
O14 U2 K1 93.75(10) . 4_645 ? 
O13 U2 K1 75.80(9) . 4_645 ? 
O5 U2 K1 48.49(9) 4_645 4_645 ? 
O17 U2 K1 107.47(13) . 4_645 ? 
O7 U2 K2 16.99(12) . . ? 
O8 U2 K2 164.08(13) . . ? 
O12 U2 K2 98.49(10) 5_655 . ? 
O14 U2 K2 72.17(10) . . ? 
O13 U2 K2 85.80(10) . . ? 
O5 U2 K2 82.27(9) 4_645 . ? 
O17 U2 K2 109.33(14) . . ? 
K1 U2 K2 130.49(3) 4_645 . ? 
O16 Se1 O9 109.17(19) . . ? 
O16 Se1 O4 108.13(19) . . ? 
O9 Se1 O4 107.72(18) . . ? 
O16 Se1 O5 113.06(19) . . ? 
O9 Se1 O5 109.41(18) . . ? 
O4 Se1 O5 109.21(17) . . ? 
O16 Se1 K2 52.72(14) . 3 ? 
O9 Se1 K2 110.48(13) . 3 ? 
O4 Se1 K2 57.27(13) . 3 ? 
O5 Se1 K2 140.11(12) . 3 ? 
O16 Se1 K3 50.55(14) . . ? 
O9 Se1 K3 58.80(13) . . ? 
O4 Se1 K3 118.19(13) . . ? 
O5 Se1 K3 132.55(12) . . ? 
K2 Se1 K3 71.71(3) 3 . ? 
O6 Se2 O2 112.1(2) . . ? 
O6 Se2 O10 111.91(18) . . ? 
O2 Se2 O10 109.06(17) . . ? 
O6 Se2 O13 109.46(19) . . ? 
O2 Se2 O13 105.50(17) . . ? 
O10 Se2 O13 108.55(19) . . ? 
O15 Se3 O11 111.9(2) . . ? 
O15 Se3 O14 110.4(2) . . ? 
O11 Se3 O14 108.60(18) . . ? 
O15 Se3 O12 113.7(2) . . ? 
O11 Se3 O12 104.99(18) . . ? 
O14 Se3 O12 106.97(19) . . ? 
O24 K1 O3 124.6(2) 2_655 . ? 
O24 K1 O6 77.17(19) 2_655 4_655 ? 
O3 K1 O6 135.36(12) . 4_655 ? 
O24 K1 O19 135.3(2) 2_655 6_566 ? 
O3 K1 O19 60.86(12) . 6_566 ? 
O6 K1 O19 134.00(13) 4_655 6_566 ? 
O24 K1 O1 65.1(2) 2_655 4_655 ? 
O3 K1 O1 84.71(11) . 4_655 ? 
O6 K1 O1 69.53(11) 4_655 4_655 ? 
O19 K1 O1 145.53(13) 6_566 4_655 ? 
O24 K1 O22 50.2(3) 2_655 2_655 ? 
O3 K1 O22 74.7(2) . 2_655 ? 
O6 K1 O22 118.11(19) 4_655 2_655 ? 
O19 K1 O22 107.56(19) 6_566 2_655 ? 
O1 K1 O22 60.8(2) 4_655 2_655 ? 
O24 K1 O8 150.1(2) 2_655 4_655 ? 
O3 K1 O8 84.64(12) . 4_655 ? 
O6 K1 O8 76.56(12) 4_655 4_655 ? 
O19 K1 O8 61.17(12) 6_566 4_655 ? 
O1 K1 O8 117.49(12) 4_655 4_655 ? 
O22 K1 O8 159.4(2) 2_655 4_655 ? 
O24 K1 N1 25.0(3) 2_655 2_655 ? 
O3 K1 N1 99.6(2) . 2_655 ? 
O6 K1 N1 96.5(2) 4_655 2_655 ? 
O19 K1 N1 125.9(2) 6_566 2_655 ? 
O1 K1 N1 57.7(2) 4_655 2_655 ? 
O22 K1 N1 25.4(2) 2_655 2_655 ? 
O8 K1 N1 172.9(2) 4_655 2_655 ? 
O24 K1 O5 129.2(2) 2_655 . ? 
O3 K1 O5 63.19(10) . . ? 
O6 K1 O5 73.05(10) 4_655 . ? 
O19 K1 O5 94.24(12) 6_566 . ? 
O1 K1 O5 66.26(10) 4_655 . ? 
O22 K1 O5 113.7(2) 2_655 . ? 
O8 K1 O5 54.13(10) 4_655 . ? 
N1 K1 O5 122.8(2) 2_655 . ? 
O24 K1 O8 77.7(2) 2_655 6_566 ? 
O3 K1 O8 142.13(11) . 6_566 ? 
O6 K1 O8 74.80(10) 4_655 6_566 ? 
O19 K1 O8 81.68(12) 6_566 6_566 ? 
O1 K1 O8 132.75(11) 4_655 6_566 ? 
O22 K1 O8 115.0(2) 2_655 6_566 ? 
O8 K1 O8 81.79(11) 4_655 6_566 ? 
N1 K1 O8 97.9(2) 2_655 6_566 ? 
O5 K1 O8 129.98(10) . 6_566 ? 
O24 K1 U2 145.81(18) 2_655 4_655 ? 
O3 K1 U2 79.34(8) . 4_655 ? 
O6 K1 U2 69.04(9) 4_655 4_655 ? 
O19 K1 U2 75.89(9) 6_566 4_655 ? 
O1 K1 U2 97.31(9) 4_655 4_655 ? 
O22 K1 U2 147.2(2) 2_655 4_655 ? 
O8 K1 U2 20.33(7) 4_655 4_655 ? 
N1 K1 U2 154.8(2) 2_655 4_655 ? 
O5 K1 U2 34.55(6) . 4_655 ? 
O8 K1 U2 97.84(7) 6_566 4_655 ? 
O24 K1 U1 118.4(2) 2_655 . ? 
O3 K1 U1 10.19(7) . . ? 
O6 K1 U1 128.74(9) 4_655 . ? 
O19 K1 U1 71.04(9) 6_566 . ? 
O1 K1 U1 74.53(8) 4_655 . ? 
O22 K1 U1 70.1(2) 2_655 . ? 
O8 K1 U1 89.45(9) 4_655 . ? 
N1 K1 U1 93.9(2) 2_655 . ? 
O5 K1 U1 59.40(6) . . ? 
O8 K1 U1 152.21(8) 6_566 . ? 
U2 K1 U1 80.93(3) 4_655 . ? 
O22 K2 O16 122.2(2) . 4_645 ? 
O22 K2 O18 91.0(2) . 5_665 ? 
O16 K2 O18 134.06(14) 4_645 5_665 ? 
O22 K2 O7 117.0(2) . . ? 
O16 K2 O7 69.65(12) 4_645 . ? 
O18 K2 O7 66.92(13) 5_665 . ? 
O22 K2 O20 154.2(2) . . ? 
O16 K2 O20 75.33(16) 4_645 . ? 
O18 K2 O20 87.19(16) 5_665 . ? 
O7 K2 O20 85.77(15) . . ? 
O22 K2 O16 93.9(2) . 3_445 ? 
O16 K2 O16 64.45(14) 4_645 3_445 ? 
O18 K2 O16 151.17(13) 5_665 3_445 ? 
O7 K2 O16 133.53(12) . 3_445 ? 
O20 K2 O16 76.31(15) . 3_445 ? 
O22 K2 O4 79.4(2) . 3_445 ? 
O16 K2 O4 115.49(11) 4_645 3_445 ? 
O18 K2 O4 100.05(12) 5_665 3_445 ? 
O7 K2 O4 157.99(12) . 3_445 ? 
O20 K2 O4 75.61(14) . 3_445 ? 
O16 K2 O4 53.26(10) 3_445 3_445 ? 
O22 K2 O21 61.9(2) . 5_665 ? 
O16 K2 O21 85.43(14) 4_645 5_665 ? 
O18 K2 O21 84.07(14) 5_665 5_665 ? 
O7 K2 O21 57.90(13) . 5_665 ? 
O20 K2 O21 143.15(16) . 5_665 ? 
O16 K2 O21 123.02(13) 3_445 5_665 ? 
O4 K2 O21 141.19(13) 3_445 5_665 ? 
O22 K2 Se1 90.6(2) . 3_445 ? 
O16 K2 Se1 88.34(9) 4_645 3_445 ? 
O18 K2 Se1 125.17(11) 5_665 3_445 ? 
O7 K2 Se1 150.86(9) . 3_445 ? 
O20 K2 Se1 69.86(12) . 3_445 ? 
O16 K2 Se1 26.54(7) 3_445 3_445 ? 
O4 K2 Se1 27.39(6) 3_445 3_445 ? 
O21 K2 Se1 141.63(11) 5_665 3_445 ? 
O22 K2 K2 82.4(2) . 2_655 ? 
O16 K2 K2 44.89(9) 4_645 2_655 ? 
O18 K2 K2 166.37(10) 5_665 2_655 ? 
O7 K2 K2 105.57(10) . 2_655 ? 
O20 K2 K2 103.96(13) . 2_655 ? 
O16 K2 K2 41.89(8) 3_445 2_655 ? 
O4 K2 K2 90.45(8) 3_445 2_655 ? 
O21 K2 K2 82.30(11) 5_665 2_655 ? 
Se1 K2 K2 67.06(4) 3_445 2_655 ? 
O22 K2 K3 136.4(2) . 3_445 ? 
O16 K2 K3 42.92(8) 4_645 3_445 ? 
O18 K2 K3 129.44(10) 5_665 3_445 ? 
O7 K2 K3 96.26(8) . 3_445 ? 
O20 K2 K3 42.89(13) . 3_445 ? 
O16 K2 K3 43.22(8) 3_445 3_445 ? 
O4 K2 K3 78.11(7) 3_445 3_445 ? 
O21 K2 K3 128.31(11) 5_665 3_445 ? 
Se1 K2 K3 55.01(2) 3_445 3_445 ? 
K2 K2 K3 61.08(3) 2_655 3_445 ? 
O22 K2 U2 123.3(2) . . ? 
O16 K2 U2 59.14(9) 4_645 . ? 
O18 K2 U2 76.58(10) 5_665 . ? 
O7 K2 U2 10.74(8) . . ? 
O20 K2 U2 81.23(12) . . ? 
O16 K2 U2 122.79(8) 3_445 . ? 
O4 K2 U2 156.76(8) 3_445 . ? 
O21 K2 U2 61.92(10) 5_665 . ? 
Se1 K2 U2 141.35(4) 3_445 . ? 
K2 K2 U2 97.10(5) 2_655 . ? 
K3 K2 U2 86.36(3) 3_445 . ? 
O23 K3 O23 11.9(4) 3_545 4_645 ? 
O23 K3 O20 110.9(3) 3_545 4_655 ? 
O23 K3 O20 107.7(3) 4_645 4_655 ? 
O23 K3 O20 107.7(3) 3_545 3 ? 
O23 K3 O20 110.9(3) 4_645 3 ? 
O20 K3 O20 141.1(2) 4_655 3 ? 
O23 K3 O16 143.2(2) 3_545 . ? 
O23 K3 O16 154.4(2) 4_645 . ? 
O20 K3 O16 71.81(14) 4_655 . ? 
O20 K3 O16 75.10(14) 3 . ? 
O23 K3 O16 154.4(2) 3_545 2_755 ? 
O23 K3 O16 143.2(2) 4_645 2_755 ? 
O20 K3 O16 75.10(14) 4_655 2_755 ? 
O20 K3 O16 71.81(14) 3 2_755 ? 
O16 K3 O16 62.32(15) . 2_755 ? 
O23 K3 O24 44.3(3) 3_545 3_545 ? 
O23 K3 O24 48.4(3) 4_645 3_545 ? 
O20 K3 O24 155.2(2) 4_655 3_545 ? 
O20 K3 O24 63.5(2) 3 3_545 ? 
O16 K3 O24 125.88(19) . 3_545 ? 
O16 K3 O24 126.9(2) 2_755 3_545 ? 
O23 K3 O24 48.4(3) 3_545 4_645 ? 
O23 K3 O24 44.3(3) 4_645 4_645 ? 
O20 K3 O24 63.5(2) 4_655 4_645 ? 
O20 K3 O24 155.2(2) 3 4_645 ? 
O16 K3 O24 126.9(2) . 4_645 ? 
O16 K3 O24 125.88(19) 2_755 4_645 ? 
O24 K3 O24 92.2(3) 3_545 4_645 ? 
O23 K3 O9 93.8(2) 3_545 . ? 
O23 K3 O9 105.6(2) 4_645 . ? 
O20 K3 O9 105.47(14) 4_655 . ? 
O20 K3 O9 67.74(14) 3 . ? 
O16 K3 O9 52.29(9) . . ? 
O16 K3 O9 108.87(10) 2_755 . ? 
O24 K3 O9 79.6(2) 3_545 . ? 
O24 K3 O9 114.4(2) 4_645 . ? 
O23 K3 O9 105.6(2) 3_545 2_755 ? 
O23 K3 O9 93.8(2) 4_645 2_755 ? 
O20 K3 O9 67.74(14) 4_655 2_755 ? 
O20 K3 O9 105.47(14) 3 2_755 ? 
O16 K3 O9 108.87(10) . 2_755 ? 
O16 K3 O9 52.29(9) 2_755 2_755 ? 
O24 K3 O9 114.4(2) 3_545 2_755 ? 
O24 K3 O9 79.6(2) 4_645 2_755 ? 
O9 K3 O9 160.62(13) . 2_755 ? 
O23 K3 N1 22.1(3) 3_545 3_545 ? 
O23 K3 N1 28.8(3) 4_645 3_545 ? 
O20 K3 N1 132.7(2) 4_655 3_545 ? 
O20 K3 N1 85.7(2) 3 3_545 ? 
O16 K3 N1 135.7(2) . 3_545 ? 
O16 K3 N1 146.6(2) 2_755 3_545 ? 
O24 K3 N1 22.6(3) 3_545 3_545 ? 
O24 K3 N1 70.5(3) 4_645 3_545 ? 
O9 K3 N1 83.6(2) . 3_545 ? 
O9 K3 N1 114.7(2) 2_755 3_545 ? 
O23 K3 N1 28.8(3) 3_545 4_645 ? 
O23 K3 N1 22.1(3) 4_645 4_645 ? 
O20 K3 N1 85.7(2) 4_655 4_645 ? 
O20 K3 N1 132.7(2) 3 4_645 ? 
O16 K3 N1 146.6(2) . 4_645 ? 
O16 K3 N1 135.7(2) 2_755 4_645 ? 
O24 K3 N1 70.5(3) 3_545 4_645 ? 
O24 K3 N1 22.6(3) 4_645 4_645 ? 
O9 K3 N1 114.7(2) . 4_645 ? 
O9 K3 N1 83.6(2) 2_755 4_645 ? 
N1 K3 N1 50.0(4) 3_545 4_645 ? 
U1 O1 K1 149.09(19) . 4_645 ? 
Se2 O2 U1 136.7(2) . 4_655 ? 
U1 O3 K1 153.18(17) . . ? 
Se1 O4 U1 134.8(2) . 4_655 ? 
Se1 O4 K2 95.34(16) . 3 ? 
U1 O4 K2 127.21(13) 4_655 3 ? 
Se1 O5 U2 128.16(19) . 4_655 ? 
Se1 O5 K1 133.80(17) . . ? 
U2 O5 K1 96.96(11) 4_655 . ? 
Se2 O6 K1 124.39(19) . 4_645 ? 
U2 O7 K2 152.3(2) . . ? 
U2 O8 K1 124.10(18) . 4_645 ? 
U2 O8 K1 124.34(17) . 6_565 ? 
K1 O8 K1 98.21(11) 4_645 6_565 ? 
Se1 O9 U1 137.3(2) . . ? 
Se1 O9 K3 94.44(15) . . ? 
U1 O9 K3 120.79(13) . . ? 
Se2 O10 U1 136.0(2) . . ? 
Se3 O11 U1 132.7(2) . 4_645 ? 
Se3 O12 U2 137.1(2) . 5_655 ? 
Se2 O13 U2 139.91(19) . . ? 
Se3 O14 U2 141.5(2) . . ? 
Se1 O16 K2 153.8(2) . 4_655 ? 
Se1 O16 K2 100.74(17) . 3 ? 
K2 O16 K2 93.22(12) 4_655 3 ? 
Se1 O16 K3 103.85(16) . . ? 
K2 O16 K3 97.16(12) 4_655 . ? 
K2 O16 K3 93.76(12) 3 . ? 
U2 O17 H17A 120(5) . . ? 
U2 O17 H17B 122(4) . . ? 
H17A O17 H17B 96(6) . . ? 
K2 O18 H18A 94(5) 5_665 . ? 
K2 O18 H18B 104(4) 5_665 . ? 
H18A O18 H18B 104(6) . . ? 
K1 O19 H19A 88(4) 6_565 . ? 
K1 O19 H19B 97(4) 6_565 . ? 
H19A O19 H19B 129(6) . . ? 
K2 O20 K3 95.46(18) . 3_445 ? 
K2 O20 H20A 108(6) . . ? 
K3 O20 H20A 105(6) 3_445 . ? 
K2 O20 H20B 172(6) . . ? 
K3 O20 H20B 83(6) 3_445 . ? 
H20A O20 H20B 81(7) . . ? 
K2 O21 H21A 58(6) 5_665 . ? 
K2 O21 H21B 104(6) 5_665 . ? 
H21A O21 H21B 93(2) . . ? 
O24 N1 O23 109.5(10) . . ? 
O24 N1 O22 129.4(11) . . ? 
O23 N1 O22 120.3(10) . . ? 
O24 N1 O23 104.3(9) . 2_655 ? 
O23 N1 O23 18.6(9) . 2_655 ? 
O22 N1 O23 125.7(9) . 2_655 ? 
O24 N1 K1 62.8(6) . 2_655 ? 
O23 N1 K1 158.8(7) . 2_655 ? 
O22 N1 K1 67.5(6) . 2_655 ? 
O23 N1 K1 166.8(6) 2_655 2_655 ? 
O24 N1 K3 59.7(6) . 3_455 ? 
O23 N1 K3 51.3(5) . 3_455 ? 
O22 N1 K3 159.2(8) . 3_455 ? 
O23 N1 K3 53.9(4) 2_655 3_455 ? 
K1 N1 K3 113.8(3) 2_655 3_455 ? 
N1 O22 K2 127.8(7) . . ? 
N1 O22 K1 87.1(6) . 2_655 ? 
K2 O22 K1 110.9(3) . 2_655 ? 
O23 O23 N1 114(3) 2_655 . ? 
O23 O23 N1 48(2) 2_655 2_655 ? 
N1 O23 N1 148.3(9) . 2_655 ? 
O23 O23 K3 84.1(2) 2_655 3_455 ? 
N1 O23 K3 106.6(7) . 3_455 ? 
N1 O23 K3 97.4(5) 2_655 3_455 ? 
N1 O24 K1 92.2(7) . 2_655 ? 
N1 O24 K3 97.7(7) . 3_455 ? 
K1 O24 K3 144.4(3) 2_655 3_455 ? 
 
_diffrn_measured_fraction_theta_max    0.999 
_diffrn_reflns_theta_full              32.50 
_diffrn_measured_fraction_theta_full   0.999 
_refine_diff_density_max    2.952 
_refine_diff_density_min   -2.013 
_refine_diff_density_rms    0.226 
